AIP Conference Proceedings 2053, 030037 (2018); https://doi.org/10.1063/1.5084398 2053, 030037 © 2018 Author(s).
Increasing the resistance of a NiCrBSi
coating to heat wear by means of combined
laser heat treatment
Cite as: AIP Conference Proceedings 2053, 030037 (2018); https://doi.org/10.1063/1.5084398 Published Online: 19 December 2018
A. V. Makarov, N. N. Soboleva, M. S. Gibzun, I. Yu. Malygina, and Yu. S. Korobov
ARTICLES YOU MAY BE INTERESTED IN
Eddy-current testing of fatigue degradation in additionally heat-treated gas powder laser clad NiCrBSi coating under contact fatigue loading
AIP Conference Proceedings 2053, 040088 (2018); https://doi.org/10.1063/1.5084526
The use of intermediate inserts for CO2 laser welding of steel AISI 321 and a Grade 2 titanium alloy
AIP Conference Proceedings 2053, 030055 (2018); https://doi.org/10.1063/1.5084416
Analytical and experimental assessment of ultimate tensile strength of a hardened layer on a material surface
Increasing the Resistance of a NiCrBSi Coating to Heat
Wear by Means of Combined Laser Heat Treatment
A. V. Makarov1, 2, 3, a)
, N. N. Soboleva1, 3
, M. S. Gibzun2
, I. Yu. Malygina1
Yu. S. Korobov3
Institute of Engineering Science, Ural Branch of the Russian Academy of Sciences, 34 Komsomolskaya St., 620049, Ekaterinburg, Russia
M .N. Miheev Institute of Metal Physics, Ural Branch of the Russian Academy of Sciences, 18 S. Kovalevskoy St., Ekaterinburg, 620108, Russia
3Ural Federal University named after the first President of Russia B.N. Yeltsin, 19 Mira St., Ekaterinburg,
Corresponding author: firstname.lastname@example.org
Abstract. Testing of NiCrBSi coatings formed by gas-powder laser cladding and combined laser heat treatment, including laser cladding and high-temperature annealing, were conducted under conditions of sliding friction on the Kh12M steel according to the pin-on-disk scheme. The combined processing resulting in the formation of large carbides and chromium borides in the coatings is shown to increase their wear resistance by a factor of 1.8 at sliding velocities of 6.1 and 9.3 m/s, when there is significant frictional heating of the friction surfaces.
The formation of high-strength and wear-resistant coatings is an effective way of enhancing the performance of worn and new machine parts affected by high contact loads and temperatures. Coatings made of Ni–Cr–B–Si alloys are widely used for improving the quality of products operating under conditions of severe heating (rolls and roller beds in hot-rolling mills, hot-forming dies, parts of heat exchanging apparatuses, turbines, solid-fuel boilers, etc.) . However, heating to temperatures ranging between 700 and 1100 °С causes continuous softening and a noticeable decrease in the wear resistance of NiCrBSi plasma and laser coatings [2, 3]. In  a conclusion was made that the high-temperature use of NiCrBSi coatings is limited due to the degradation of their matrix at temperatures exceeding 700 °С.
The applicability of NiCrBSi coatings at high temperatures considerably extends the new phenomenon of increased hardness and wear resistance of laser-clad NiCrBSi coatings resulting from extra annealing at 1000 to 1075 °С, which was discussed in [4, 5]. Under annealing of the metastable structure of the laser-clad coating followed by cooling, the coating acquires a highly strong wear resistant skeleton formed by large chromium carbides and borides, which preserves its enhanced properties under heating up to the annealing temperature. Based on the discovered phenomenon, a method was developed to produce NiCrBSi coatings with extremely high (up to 1000 °С) heat resistance by combined laser heat treatment (RF patent No. 2492980) , involving laser cladding with additional high-temperature annealing. The proposed new approach to the formation of heat-resistant coatings by combined laser-thermal method (with high-temperature annealing of the clad coating) was applied to enhancing the wear resistance of nickel-based alloy specimens produced by an additive laser technique, namely, by direct laser material deposition  and to producing a coating strain-hardened by friction treatment with a sliding indenter .
However, in [4, 5, 7], the conclusion about the heat resistance of the coatings was based only on hardness and wear resistance measurements at room temperature after cooling from the annealing (tempering) temperature. The aim of this paper is to study the possibility of increasing the wear resistance of a NiCrBSi coating, under
considerable friction heating induced by sliding friction at high (above 5 m/s) speeds, by combined laser heat treatment.
MATERIAL AND EXPERIMENTAL PROCEDURE
A self-fluxing NiCrBSi powder with the composition (wt%) 18.2% Cr, 3.3% B, 4.2% Si, 0.92% С, 2.6% Fe, the rest Ni was used for cladding. The powder was clad onto a steel plate (0.20% C) with the use of a СО2 continuous
laser, with a radiation power of 1.4 to1.6 kW, a speed of 160 mm/min, a powder consumption of 2.9 to 3.8 g/min, and a 6×1.5 mm laser spot on the surface. The powder mixture composed of 40 to 160 µm grains was transported to the zone of cladding by an inert gas (argon) under a pressure of 0.5 atm. In order to decrease surface stresses, the cladding was performed in two passes by overlaying one layer onto the other. The coating thickness after cladding and polishing was 0.9 to 1.3 mm. Some specimens were subjected to combined laser heat treatment consisting in cladding followed by annealing at 1025 °С (2 hour holding) with subsequent cooling in a vacuum furnace.
Microhardness was measured on a Shimadzu HMV-G21DT microhardness tester under a load of 0.49 N as an arithmetic mean of 10 measurements. The microstructure and the wear surfaces were examined with the use of a Tescan Vega II XMU scanning electron microscope equipped with a wave dispersive (Inca Wave 700) and energy dispersive (Inca Energy 450 XT) microanalyzer.
Tribological pin-on-disk tests were performed on a laboratory device (Fig. 1). The end surfaces (7×7 mm) of the clad specimens slided on a revolving Kh12M steel disk (microhardness 61.5 HRC) in air, with the load N=98 N. The average sliding velocities were V=6.1 m/s and V=9.3 m/s, the testing time being t=22 min and t=9.5 min respectively. The testing time was determined by the linear wear of the coating, which did not exceed 0.7 mm. We determined specimen mass loss during wear, the friction force (with the use of an elastic element – a ring with resistance strain gauge transducers pasted to it) and the average temperature in the surface layer of the specimen (by a chromel-alumel thermocouple with 0.2 mm diameter electrodes welded in at a distance of ~0.5 mm from the gauge surface of the specimen).
FIGURE 1. Pin-on-disk test scheme
The wear intensity Ih was calculated by the formula Ih=Q/(ρ·S·L), were Q is specimen mass loss, g; ρ is specimen
material density, g/cm3; L is friction path length, cm; S is the geometric contact area, cm2. The friction coefficient f was determined as the friction force to normal load ratio. The linear wear was determined by the formula I=Q/(ρ·S).
EXPERIMENTAL RESULTS AND DISCUSSION
The clad NiCrBSi coating (Fig. 2a) is characterized by a fairly uniform distribution of the structural constituents across the thickness . The metal base of the coating comprises a Ni solid solution and eutectic consisting of a γ-solid solution and a Ni3B phase (Fig. 2b) [4, 8]. It was found by X-ray spectrometry microanalysis, X-ray phase
analysis  and microdurometry that chromium carbide Cr7C3 with a hardness of 1650-1800 HV and chromium
boride CrB with a hardness of 1950-2400 HV are the main strengthening phases of the coating. The average microhardness of the coating is 990 HV 0.05.
Under heating to 1025 °С followed by slow cooling in a vacuum furnace, large CrB (Fig. 2c) and Cr7C3 particles
appear in the structure of the laser coating, which form a highly strong wear resistant skeleton . Besides, there appears a new phase, namely, nickel silicide Ni2Si (Fig. 2c), which enters into the triple eutectic composition
γ+Ni3B+Ni2Si. After annealing at 1025 °С for 2 hours with slow cooling in a vacuum furnace, the average
microhardness of the coating is 1050 HV 0.05.
(a) (b) (c)
FIGURE 2. The microstructure of the NiCrBSi coating after laser cladding (а, b) and after combined processing including laser cladding and annealing at 1025 °С (c)
Table 1 presents results of tribological pin-on-disk testing of the NiCrBSi coating after laser cladding and combined laser heat treatment including laser cladding and annealing at 1025 °С (2 h holding) followed by cooling in a vacuum furnace, the tests being performed under conditions of dry sliding friction in air.
TABLE 1. Mass loss Q, wear intensity Ih, linear wear I, friction coefficient f and average temperature in the surface layer Т for coated NiCrBSi specimens in testing for sliding friction on a steel disk at various testing speeds V and testing times t
Coating state V, m/s t, min Q, mg Ih, 10-8 I, mm f Т, °С
Laser cladding 6.1 22 273.9 8.30 0.669 0.28 920
Laser cladding + annealing at 1025 °С 6.1 22 149.7 4.54 0.365 0.30 890
Laser cladding 9.3 9.5 275.3 12.74 0.672 0.20 >1000
Laser cladding + annealing at 1025 °С 9.3 9.5 150.0 6.94 0.366 0.25 >1000 The average volumetric temperature in the surface layer is seen to reach 890 °С and above in the high-speed tests. The mass loss, wear intensity and linear wear of the specimens with coatings after combined processing decrease by a factor of 1.8 from the respective characteristics of the clad coating in tests at speeds of 6.1 and 9.3 m/s. Consequently, additional high-temperature annealing of the clad coating increases significantly the frictional heat resistance of the coating, i.e. it offers a higher wear resistance under considerable frictional heating, despite the comparable values of microhardness for the laser-clad coatings and those after combined processing.
Besides, it follows from the table that the combined processing decreasing wear intensity causes no improvement of the antifriction properties of the clad coating; namely, a lower friction coefficient f is not reached, vice versa, the annealed coating demonstrates even a slight increase in the average friction coefficient. Note that, in all cases, the wear intensity of the NiCrBSi coating (see the table) is characterized by values an order of magnitude lower than those in the case of catastrophic heat-induced seizure of carbon steels after laser or bulk hardening under testing in air at speeds of 3.7 to 4.5 m/s, when the temperature of the surface layer is at most 550-700 °С [10, 11]. This testifies to increased wear resistance under considerable frictional heating of the NiCrBSi coating produced by laser cladding. Combined laser heat treatment (with annealing) offers an additional significant increase in the frictional heat resistance of the clad material.
The study of the friction surfaces testifies to the limitation of adhesive seizure and plastic edging on the wear surfaces of the additionally annealed specimens (Fig. 3). On these surfaces, under friction loading, there occurs “polishing out” of coarse strengthening phases, namely, borides CrB and carbides Cr7C3 (Fig. 3), which create a
wear resistant skeleton on the friction surfaces, which hampers the evolution of heat wearing. Similarly, the wear-resistant skeleton formed by the carbide and boride phases on the NiCrBSi coatings during testing on a fixed abrasive makes a decisive contribution to the resistance of the coatings to abrasive wear .
(c) (d) (e)
FIGURE 3. The wear surfaces of a laser-clad NiCrBSi coating (a, c) and that after combined processing including laser cladding and annealing at 1025 °С ( b, d, e) after testing for sliding friction on a steel disk at speeds of 6.1 m/s (a, b) and 9.3 m/s (c-e)
The study pioneers in demonstrating that high-temperature (1025 °С) annealing of a NiCrBSi coating produced by gas powder laser cladding decreases wear intensity and linear wear by a factor of 1.8 under conditions of sliding friction in air at sliding speeds of 6.1 and 9.3 m/s, when the temperature of the frictional heating of the surface layer reaches ~900 °С and above. The increased wear resistance is caused by the formation of coarse strengthening phases (chromium borides CrB and chromium carbides Cr7C3 in the coating under annealing, which hamper the evolution
of heat-induced seizure and plastic edging. Thus, combined laser heat treatment including laser cladding and high-temperature annealing increases the frictional heat resistance of the NiCrBSi coating.
The work was done within the state assignment from FASO Russia on the subject “Structure”, No. AAAA-A18-118020190116-6 and the state assignment for IES UB RAS, subject No. AAAA-A18-118020790147-4. The experimental research was done on the equipment installed at the Plastometriya collective use center of IES UB RAS.
1. Ch. Guo, J. Zhou, J. Chen, J. Zhao, Y. Yu and H. Zhou, Wear 270, 492–498 (2011).
2. A. Zikin, M. Antonov, I. Hussainova, L. Katona and A. Gavrilović, Tribol. Int. 68, 45–55 (2013).
O. I. Shevchenko, V. M. Farber and G. E. Trekin, Izvestiya VUZov: Chernaya Metallurgiya 10, 76–
4. A. V. Makarov, N. N. Soboleva, I. Yu. Malygina and A. L. Osintseva, Met. Sci. Heat Treat. 57 (3–4), 161–168 (2015).
5. A. V. Makarov, N. N. Soboleva, I. Yu. Malygina and A. L. Osintseva, R. F. Patent No. 2492980 (2013). 6. A. I. Gorunov and A. Kh. Gilmutdinov, Int. J. Adv. Manufact. Techn. 86, 2567–2574 (2016).
7. A. V. Makarov, N. N. Soboleva and I. Yu. Malygina, “Thermal stability of a laser-clad NiCrBSi coating hardened by frictional finishing,” in Mechanics, Resource and Diagnostics of Materials and Structures, MRDMS 2017, AIP Conference Proceedings 1915, edited by E. S. Gorkunov, V. E Panin, S Ramasubbu (American Institute of Physics, Melville, NY, 2017), pp. 030012.
8. A.V. Makarov, E.S. Gorkunov, I.Yu. Malygina, L.Kh. Kogan, R.A. Savrai and A.L. Osintseva, Russ. J. Nondestr. Test. 45, 797–805 (2009).
9. N.N. Soboleva, A.V. Makarov and I.Yu. Malygina, J. Physics: Conf. Series 946, 012004 (2018). 10. A.V. Makarov, L.G. Korshunov, I.Yu. Malygina and I. L.Solodova, Met. Sci. Heat Treat. 49 (3–4), 150–156
11. A.V. Makarov, L.G. Korshunov, V.B. Vykhodets, T E. Kurennykh and R.A. Savrai, Phys. Met. Metallogr. 110 (5), 507–521 (2010).